21.Dry or Chemical Corrosion It is the degradation of a material due to a reaction with its environment.ORProcess of Distruction of the material through chemical or electrochemical attack by its environment.Slow processMeasured in weight loss per unit time.Classification:Dry or Chemical CorrosionWet or Electrochemical corrosion1.Dry or Chemical CorrosionOccurs due to chemical attack of by the environment such as dry gas.Occurs due to high temperature and without liquid phase.
3(a)Oxidation Corrosion: It is of two types:a) Oxidation corrosion b) Corrosion by gases(a)Oxidation Corrosion:It is due to direct attack of oxygen on metals.Oxygen molecules are attracted to the surface by Vander Wall ForceMechanism:-1. When temp increases the metal undergoes oxidation and losses e-2M → 2M+n ne-Metal Ion2. Electron are gained by the oxygen molecules forms oxide ionsnO2 + 4ne- → 2n O2-Oxide Ion3. Scale of metal oxide formed2M + nO2 → 2M + 2n O2-Metal Oxide
42. Wet or Electrochemical Corrosion Stable Corrosion: -Aluminium, Tin, Lead, CopperNon-stable corrosion:- Silver, Gold, PlatinumPilling – Bed Worth RatioRatio of volume of oxide formed to the volume of metal consumed.(b)Corrosion by GasesCarbon di-oxide, Chlorine, Hydrogen Sulphide, Sulphur di-oxide, FlourineDepends on chemical affinity b/w metal and the gas.2. Wet or Electrochemical CorrosionOccurs when aqueous solution or liquid electrolytes are presentWet corrosion takes place in environments where the relative humidity exceeds 60 %.Wet corrosion is most efficient in waters containing salts, such as NaCl (e.g. marine conditions), due to the high conductivity of the solution.
5Mechanism Of Electrochemical Corrosion Anodic Reaction:Dissolution of metal takes place.As result metal ions are formed with the liberation of free electrons.M ↔ M+n e-Metal Ion
6Cathodic ReactionHydrogen Evolution :- Occurs usually in acidic medium2H+ + 2e- ↔ H2 (g)(ii) Oxygen Absorption :- occurs when solution is aerated sufficiently.O2+ 4H+ + 4e- ↔ 2H2O (In acidic medium)O2+ 4H+ + 4e- ↔ 4OH- (In basic medium)Forms of Corrosion:Galvanic Corrosion:- When two different metals are present in contact with each other in conducting medium e.g. Electrolyte
7(b) Concentration Cell Corrosion:- Same as Galvanic corrosionOccurs when two different metals are exposed to different air conc.(c) Pitting Corrosion:-Formed as a result of pit and cavitiesLocalized attack and formed by cracking protective coating
8For Class Test I (d) Stress Corrosion: Occurs in the presence of tensile stress and corrosive environmentE.g. brass get corrode in traces of ammonia.For Class Test I
9Factors Affecting Corrosion Nature of the Metal Nature of the environment.Nature of MetalPosition in Galvanic Series:If two metals are present in in electrolyte, the metal with less reduction potential undergoes corrosion.Greater the difference faster the corrosion.(ii) Over Voltage:Due to high evolution of hydrogen, the rate is slow.(iii) Area and Distance:When anodic metal area is smaller than cathodic area, rate of corrosion at anode is higher because of demand of electron by cathodic area.
10(iv) Physical and Mechanical properties of Metal: Pure metals are more corrosion resistant.Smaller grain size metal have high solubility and corrosion.Uniform distribution of stress on metal reduces rate of corrosion.Passive metals shows higher corrosion resistance because of formation of protective oxide film on their surface.Polycrystalline forms are more sensitive.2. Nature of EnvironmentTemperature: directly proportionalHumidity: faster in humid conditionspH : If less than 7 rate is high. Al, Zn, Sn, Pb, and Fe are affected by both acid and bases.Impurities and Suspended Particles: When these will get dissolved in moisture, provides electrolyte for conductivity and hence corrosion increases.
11Corrosion Control:Selection of metal and alloy:Using pure and noble metalsPractically not possible because of low strength of pure metalUse of metal alloys which are homogeneous2. Proper design of metal:Minimal contact with mediumPrevention from moistureAdequate ventilation and drainageWeldingAvoid cervices b/w adjacent partsBend should be smoothBimetallic contacts should be avoidedPaint cathodic portionPrevent uneven stress
123. Cathodic Protection:Force the metal to be protected to behave like cathode.Sacrificial anodic protection:Metal to be protected from corrosion connected to more anodic metalCommonly used metals Mg, Zn, Al and their alloysImpressed current method:Direct current is applied in opposite direction to nullify the corrosion currentConverts the corroding metal from anode to cathode.
134. Modifying Environment Eliminating dissolved oxygen:De-aerationBy using chemical substances like sodium sulphite and hydrazine. Also called Deactivation.Reducing Moisture:Dehumidification by using silica gelsReducing Acidity:Neutralizing the acidic environment by adding lime, NaOH, AmmoniaCommonly used in refineries5. Protective coating:Application of coatingCoating material should be chemically inert under particular temp and pressure.
146. Use of corrosion Inhibitor Anodic Inhibitor:These are oxygen and oxidizing agent.They combine the anodic metal forming an oxide film which reduce corrosionCathodic Protection:Organic inhibitors like amines, mercaptans, urea and thiourea reduces the H ion diffusion by adsorptionMercury, arsenic and antimony deposits films at cathodic area which raise the hydrogen over volume.Eliminating Oxygen from the medium by adding sodium sulphate and hydrazine.
16Protective CoatingSurface preparation for Coating:Cleaning:To prepare for suitable conditionRemoving contaminants to prevent detrimental reaction productE.g. de-greasing, sand blasting, vapour degreasing, pickling and alkaline cleaning.Solvent Cleaning:Must be non-inflammable and nontoxicTrichloro trifluoroethane which has low toxicity are costlierVapour de-greasing is economical and advantageous because of continuous cleaning with small quantities of solvent.Electrolyte Pickling:Provides better and rapid cleaning by increasing hydrogen evolution resulting in agitation and blasting actionSand blasting is mechanical cleaning.
174. Alkaline Cleaning:Cheaper and less hazardousUsed in conjunction with surface active (wetting) agentAbility depends on pH, rapidly decreases below 8.5Other abilities are rinsability, detergent properties, sequestering, wetting etc.Acid CleaningAcid such as HCl, H2SO4, H3PO4 is very effective.5-10% H2SO4 and HCl used to remove inorganic contaminants.Pickling are performed at high temp. (60 ̊C)Is effective for removal of grease, oil , dirt and rust.
18Methods of Application of Metallic Coating Hot Dipping:Metal is kept in molten state and base metal is dipped into it.Used for producing a coating of low M.PE.G. Tinning (Tin coating on Iron)Process is followed by cooling the coating through a palm oil to prevent oxidation of tin plate to its oxide.Palm oil layer is removed by alkaline cleansing agent.Metal Cladding:The surface to be protected is sandwiched between two layers of the coating metals and pressed between rollers.E.g. Alclad Sheeting– Plate of duralumin is sandwiched between 99.5%pure aluminum
193. Electro Plating:Pure metal is made as cathode and base metal as anode.Electrochemically coat metal is deposited on base metal.This metal gives smooth, fine and uniform coatingIt depends on(i) Temperature (ii) Current density (iii) Electrolyte ConcentrationNature of base metal (v) Time4. Electroless Plating:Nobel metal is deposited catalytically on less noble metal by using reducing agent without using electrical energy.Advantage over Electro platingMore economical since no electricity requiredIrregular shape can be plated uniformlyPlating on plastics can also be done
20Chemical Conversion Coating 5. Metal Spraying:Coating is applied by means of spraying deviceE.g. Aluminum is plated in this way on Aircrafts.Chemical Conversion CoatingThese are formed on metal surface by chemical reaction b/w metal surface and inorganic salt solutionCoating base metal is converted into one of the resultant protective film.These films are insoluble, adherent, crystalline or amorphous in nature.Can be done in 3 waysPhosphate coatingChromate coatingAnodized coating
21Phosphate CoatingProduced by chemical reaction b/w base metal and aq. H3PO4, Zn or Fe or Mn PhosphatePhosphate coating are applied Iron, Steel, and ZincFilm formed on base metal after coating consist of Zn-Fe, Mn-Fe Phosphates.Chromate CoatingProduced by dipping the base metal in Potassium chromate (acidic) followed by immersion in neutral chromate bath.Resulting film consist of trivalent and hexavalent chromium.Used as base for paints, lacquers and enamels.
223. Anodized CoatingFormed by anodic oxidation processThis is produced on non-ferrous metals like Al, Zn, MgIn this method base metal is made as anodeProcess is carried out by passing moderate direct current through a bath in which the metal is suspended as anode.Coating are formed as a result of Progressive oxidation starting at surface of base metal.